Research Inventy: International Journal Of Engineering And ScienceVol.2, Issue 8 (March 2013), Pp 11-17Issn(e): 2278-4721, Issn(p):2319-6483, Www.Researchinventy.Com11Damage Characterization of a Thin Plate Made Of ABS underUniaxial SolicitationH. Farid1, K. Elhad1, M. Elghorba1,F. Erchiqui2, M. Chergui11.Laboratoire De Bioplasturgie Et Nanotechnologie, Université Du Québec Abitibi-Témiscamingue, 445Boulevard De l’Université, Rouyn-Noranda, Québec J9X 5E4, Canada2.Laboratoire De Contrôle Et Caractérisation Mécanique Des Matériaux Et Des Structures, École NationaleSupérieure d’Électricité Et De Mécanique, Route dEl Jadida. BP 8118 Oasis Casablanca, MarocAbstract: There is an important soaring in theuse of polymers in many industrial fields. Although they areabundantly used both in ordinary and high performance products, their versatility makesthem highly needed fornewer applications; and thisrequires a detailed knowledge of their physical, chemical, rheological andmechanical properties. The determination of mechanical behavior of those materials becomes very necessaryeither during processing or under operation. In this work, we are interested in characterizing a notchedpolymeric ABS flat plate under uniaxial solicitation. TheUnified Damage Theory for characterizing andquantifying the damage is used. Our crucial aim, being thestudy of the stress concentration factor,and acontribution to the determination of the damage degree of notched structures.Key words: Damage mechanics, Damage theory, Uniaxial characterization, Softened polymer, ABS.I. INTRODUCTIONMany engineering studies show that whatever the material (metal, polymers, composites, or wood),inspite of their various microstructures and physical properties, the qualitative mechanical behavior they exhibit issubstantially identical. These include an elastic behavior, a yield stress, certain plasticity or irreversibledeformation, more or less important deformation anisotropy, a hysteresis ring with damage by monotonic orcyclic loading, and a crack initiation under static or dynamic loading .Additionally, they exhibit many levelsof imperfections, due to processing, post processing handling such as transportation and storage. Suchimperfections include knit lines, flaws, vacuum or inclusions which make polymer-based structuresheterogeneous to a certain degree.The consequences of the presence of knit lines for example in such materials on the mechanicalproperties are discussed by Criens and Moslé . Due to the presence of crazes, scratches, cracksand otherimperfections, the mechanical properties of realpolymeric materials are not as good as they theoretically couldbe .Damage mechanics aimsat modeling these phenomena at the level of structures calculations. The purposeof this approach being to build behavior models which once included in a calculation code,could simulate thefracture and, more generally, to estimate the state of damagesin a structure according to one or many ultimatestates .Modeling the structural behavior of polymers has been the subject of a range of researches. In thisregard, several authors have addressed the problem of rheological behavior , formingand processingmodeling , and the behavior during the failure process .This work is a contribution to the study of thefailure mechanism of a flat plate made by ABS (Acrylonitrile-Butadiene-Styrene). Initially, the structuralbehavior of a smooth plate has been studied, in aim to study and reveal the mechanical characteristic underuniaxial solicitation tensile test, followed by a series of tests conducted on notched flat plates, the notch effectwill be discussed and highlighted through experimental results. Finally, through the application of the stressconcentration factor criteria , and the Unified Damage Theory , the damage evolution in the ABS materialis investigated.II. THEORYGenerally, damage decreases the stiffness and resistance of materials. For a given stress state, thedeformations are all larger than the damage is high. Hence the importance of coupled calculations, whichcalculates simultaneously stress, strain and damage in mechanical properties evolution problems.The main aimof damage theories is to define a Damage parameter which translates the damage state of the structure.However, it remainsa delicate problem since nothing (or almost nothing!) distinguishes a damaged volumeelement of a virgin (blank)volume element macroscopically. It is then necessary to imagine an internal variablerepresenting the state of deterioration of the material.
Damage Characterization Of A Thin Plate Made...12Several modelsare proposed for damage modeling in structural calculation.The most responded modelis theMinner model of damage , , however it remains limited in its linear method of description of thecumulative damage progress, which does not accurately reflect the state of the deterioration of the structure.Other proposed approaches have tried to adjust this model to a more adequate damage presentation;they includethe models of Miller  and Chaboche …In order to address the various points omitted by the theoretical damage models, Bui-Quoc proposeda model that involves several loading parameters. The Unified Theory hasthus been developed in this context, todefine damageparameter which is the internal variable that describe the damage state of the structure in terms ofthe a life fraction , the fraction of life depends on solicitation conditions (for example the number ofcycle for dynamics loading, notch dimension for static tensile loading, temperature conditioning…).In thisrespect, the endurance limit is defined as the stress level below which there is no damage, the part supports aninfinite number of cycles in fatigue tests for example, or its resistance reach the highest level for a notched statictest specimen. The rate of reduction of the endurance limitto the number of applied fatigue cyclesfor a dynamicsolicitation test was suggested as follows:(1)Wherethe various terms are successively:Non-dimensionalendurencelimitNon-dimensionalcyclic stressInstantaneous non-dimensional endurance limitEndurance limit of the virgin materialApplied stress leveland Material constantsNumber of applied fatigue cyclesWith boundary conditions:i.ii.Where is the number of cycles to failure for a fatigue test; for our study, it represents the critical diameter ofthe hole, m is an empirical material constant superior to one.(2)WithThis equation determines the relationship between stress and applied number of cycles. The normalized damageis defined by:(3)WithBy setting posing this theory leads to the following equation:(4)For the damage quantification in the material, we used the damage variable for each life fraction, so byanalogy with theory shown above, the life fraction of our study representsthe relationship between the holediameter progressionand its critical value, which is the value of the larger hole diameter. Based on the earlierpresented theories, we chose the law of damages given by the unified theory. The mean advantage of this theoryrelative to other approaches is to directly link the damage progressof the material to the variation of the ultimateresidual limit, thus directly connecting the material’s damage to its characteristics.Thedamage variable can thusbe defined as:
Damage Characterization Of A Thin Plate Made...13(5)Whereis theultimate residual stressis the ultimate limit,is the stress limitIII. ExperimentalA series of tests was carried on forthe characterization of material damage, on two series ofrectangularspecimensofABS (Acrylonitrile-Butadiene-Styrene), based on theguidelines prescribed by the ASTM D 882-02 and ASTM D5766M . Thefirst series consisted ofrectangular smooth specimens (without hole) tocharacterize the materialand the second series consisted of rectangular specimens with holes of 1 mm to7mmdiameters. The first series was used as the reference, and the second to monitorandhighlight the influenceof the hole size on the specimenbehavior. All the experimental series was conducted under controlleddisplacement. Elongations were determined using the displacement sensor crosshead incorporated in themachine. Figure 1 below shows the set-up for the tensile test.Figure 1. Experimental set-up:A test specimen held by the sample holder of the tensile testing machine (left),anddimensions of the test specimen (right).IV. RESULTSIn the notched specimen, a stress concentration phenomenon near the hole takes place, and the responseof the structure to the applied effort is affecteddepending on the hole diameter, we talk here on a notch effect.Figure 2 shows the stress versus strain curves for the specimens with holes.As the tests proceed, these curvesshow a strikingdecreasing pace, and the gap between the values.Figure 2. Evolution of the stress-strain curves foruniaxial tensile tests on rectangular test specimens with 1mmto 7mm hole diameters, according to ASTM D 882-02 two and ASTM D5766M
Damage Characterization Of A Thin Plate Made...14In fact, these curves showa remarkable degradation of the mechanical properties of the material with anincrease in hole diameter; these properties include the elastic stress, ultimate stress, the failure stress and theelongation.We observe an area of stress stabilization, and a high elongation (maximum elongation).Additionally, rupture is often preceded by local yielding followed byanabrupt failure.The mechanicalcharacteristics are affected due to the notch effect; the characteristics decrease as long as the notch diameterincreases. Figures 3 showsthe evolution of the ultimate stress thewithhole diameter:Figure 3. Ultimate stress evolution withhole diametersFigure 4. Stiffness evolutionwithhole diametersAs already mentioned above, a decrease in the ultimate stress (maximum stress value reached in thetensile test) with hole diameters was observed.The right branchof the stress-strain curve present the elasticresponse of the specimen, this branch allows the calculation of the Young Modulus. However, with the existenceof the hole, we talk more about Stiffnessfor notched specimens’more than Young modulus for smooth specimens.The stiffness determines then the elastic response limits for notched structures. Figure 4 shows a significant risein stiffness until values closer to those given by smooth specimens which represent the Young’s modulus.Asdiscussed above, the existence of notch affect the mechanical characteristics of the material, the evolution of itssize has also remarkable influence on those properties. Figure 5 shows aschematicalevolution of the ultimatenondimensional stress versus nondimensional hole diameter.The ultimate nondimensional stress was obtainedby nondimensionalization of the ultimate residual stress (the residual ultimate stress is given as the ultimatevalue of stress reached by a sane specimen in a simple tensile test, for our study, its value is ) bythe ultimate stress level obtained for each hole diameter.The same for the nondimensional hole diameter whichwas obtained by nondimensionalization of the hole diameter by the critical hole diameter (the larger value of thehole diameter above which the structure no longer support any effort).
Damage Characterization Of A Thin Plate Made...15Figure 5. Evolution of the ultimate nondimensional stress versus the nondimensional hole diameterFigure 5 illustratesthe ultimate nondimensional stress evolution versus thenondimensionalholediameter; thecurve shows a decrease of the material ultimate stress while the nondimensional hole increases. The intersectionwith the interval limit allows us to determine a stress limit below which we estimate that the damage occurred tothe material remains acceptable, this stress limit has as value .Figure 6 reports the variation ofthe resistance loss with the nondimensional diameter of the holes. It shows that the resistance loss is remarkableand it becomesincreasingly important when approaching the critical value of the default already prescribed.Theaim of this representation is to show the resistance loss of the material due to the damage accumulation, thisdamage itself is due to the notch and its evolution in the structure.Fatigue behavior of thematerial,ascharacterized through its endurance limit,allows us to determine the endurance limit that will be usedlater for the quantification of the material damage. The endurance limit was determines for the ABS smoothsamples, throughfatigue test, and takes as value .Figure 6. The resistance loss in static tensionBoth curves of Figure 6 have the same shapelike the one giving the variation of the ultimate limit. Bothshow a resistance decrement while the nondimensional hole diameter keep increasing. Theintersection betweenthe later curve andthe boundary of the interval of study gives a value which is considered thesafeendurance limitvaluebelow which nofatigue failure will occur.
Damage Characterization Of A Thin Plate Made...16V. DAMAGE IN THE ABS NOTCHED PLATESFigure 7. Evolution of the damage versus the fraction of lifeFor quantifying the damage occurred into the notched structure, we propose a damage variable basedon presentation demonstrated above in equation (5). The proposition of this variable was taken by analogy withcumulative damage theory proposed by Gatts  and retaked by Bui-Quoc . The proposed approach presentthe damage evolution into a notched structure, and link the damage state of the material to an intrinsic propertywhich is its residual stress.The damage on the notched samples with the non-dimensional hole diameters isshown in the figure 7. The damagenearlyfollowsa linear variation.At theinitiation, the damage isnegligible for a smooth flat plate. As the hole size increases,the damage acceleratesa maximum value of0.9is reached where failure occurred.The initiation area is characterized by the highest mechanicalcharacteristics for the materials, while the point of failure is marked by their remarkable degradation.VI. STRESS CONCENTRATION IN THE NOTCHED ABS PLATESThe concept of a stress concentration factor is often employed by designers to account for the increaseof stress at a concentration point, the nominal stress being multiplied by a stress concentration factor to obtainand estimate of the local stress at the point.Generally, Stress concentration is a phenomenon of a local stressincreasing in an area which contains geometric modifications .It appears in a discontinuity of a part or astructure for examplewith the presence of a notch after machining. The area of stress concentration is most oftenthe site of crack initiation.In many cases, particularly in which the stress is highly localized, a mathematicalanalysis proves difficult or impracticable. Then, experimental or mechanical methods of stress analysis are used.The vicinity of the incident formis characterized by a heterogeneous stress distribution leading to the stressconcentration, thus stress concentration factor is defined as “the quotient of the maximal applied stress to thecorresponding nominal stress” :(6)The severity of the stress concentration depends on both the notchgeometry and the notchconfiguration. Stressconcentration is an important factor to be considered during every structural design, as issues such as suddenbreak can be avoided either by reducing or by avoiding it .The stress concentration factor variation relative to the specimen ratio hole diameter to width is shown in thefigure 8.
Damage Characterization Of A Thin Plate Made...17Figure 8.Evolution of the stress concentration factor with the hole diameterbased on the ratio D/W for notchedplateThestress concentration factor decreases with the ratio D/W.This means that stress concentration increases witha reduction of D/W.Additionally, this concentration tends towards stability when the ratio D/W increases, thusthe maximum stress is equal to the nominal stress, and the large size of the defect has no effect on this ratio.VII. CONCLUSIONThe objective of this work was to characterize the damage behavior of a thermoplastic flat plate. Itfound that the uniaxial tensile test was the most practical approach and the closest representation of the real stateof deformation during the real solicitation.Thistechnique was used to describe the damage occurring to thematerial. The unified damage theory was used in the aim to give a more complete damage model that can morefaithfully describe the state of the material. This approach was applied to several materials; however the resultsreported in this article are only based on ABS.The results obtained have highlighted the applicabilityof thereporteddamage approach. The proposed approach involves the use of theintrinsic parameters ofthematerial,thusa rigorous description of the damage state of the materials. These preliminary studies are essential stepstowards the full achievement of our mid-term goals of performing and developing tools for modeling andsimulatingof thermoplastic forming processes.REFERENCES Sanchez-Santana U., Comportement dynamique des matériaux et structures après sollicitation en fatigue. Thèse de doctorat,Université des sciences et technologies de Lille, 2007. Criens R.M. and Moslé H.G., Faillure of plastics, edited by W. Brostow and R.D. Corneliunssen Hauser, 1986. Brostow W., Kubàt J. and Kubàt M., Physical properties of polymers handbook, Chapter 23: Mechanical properties, AmericanInstitute of physics, James E. Mark editor, 1996. Lemaitre J. andChaboche J.L., Aspect phénoménologique de la rupture par endommagement, journal de la mécanique appliquée,Vol 2, 1978. Shia-Chung C., Rheologicalbehavior of PS polymer melt under ultra-high speed injection molding, Polymer Testing Journal,Volume 31, Issue 7, October 2012. Erchiqui1 F., Ozdemir Z., Souli M., Ezzaidi H., Dituba-Ngoma G., Neural networks approach for characterization of viscoelasticpolymers, volume 89, Issue 5, October 2011. Figueredo R., Cherouat A., Une nouvelle approche dans la prise en compte de la déformation permanente et volumique induite parl’endommagement dans la mise en forme des structures caoutchoutiques, 19 ème Congrès Français de Mécanique, Marseille 2009. Davis J.R., Tensile testing second edition, ASM International, The material information society 2004. Bui-Quoc T., Dubuc J., Bazergui A., Biron A., Cumulative fatigue damage under stress-controlled conditions, Journal of BasicEngineering, Transactions of the ASME, 1971. Miner M., Cumulative damage in fatigue, Journal of Applied Mechanics, Volume 12, 1945. Jardin A., Leblond J.B., Berghezan D., Par-delà la loi de Miner pour la modélisation de la fatigue des élastomères : théorie etexpérimentation, 19 ème Congrès Français de Mécanique, Marseille 2009. Miller K.J., Zachariah K.P, Cumulative damage fatigue crack initiation and state I propagation, Journal of Strain Analysis, 1977. Lemaitre J, Chaboche J.L, Mechanics of Solid Materials, Cambridge University Press, Cambridge, UK, 1990. D 882-02 ASTM Standard test method for tensile properties of thin plastic sheeting. D5766M ASTM Standard test method for open hole tensile strength of polymer matrix composite laminates. E606 / E606M - 12 ASTM Standard Test Method for Strain-Controlled Fatigue Testing. Gatts R., Application of cumulative damage concept to fatigue, ASTM Transactions, Journal of basic engineering, Volume 83,1961. LemaignanC., La Rupture des matériaux, EDP Sciences 2003. Boresi A.P., Sidebottom O.M., Advanced mechanics of materials 4thedition, John Wiley and sons 1985. Lemaitre J, Chaboche J.L, Mécanique des matériaux solides 3èmeédition, Edition Dunod 2009.